Available online at www.sciencedirect.com
Ceramics International 35 (2009) 3407–3410 www.elsevier.com/locate/ceramint
Preparation of Ni-coated Si3N4 powders via electroless plating method Jinhui Dai a,*, Xizhong Liu a, Huazhang Zhai b, Zhongfang Liu a, Jintao Tian a a
Institute of Materials Science and Engineering, Ocean University of China, Songling Road 238, Qingdao 266100, Shandong Province, PR China b School of Materials and Engineering, Beijing Institute of Technology, Beijing 100081, PR China Received 9 April 2009; received in revised form 4 May 2009; accepted 11 June 2009 Available online 7 July 2009
Abstract The Ni/Si3N4 coated powders were successfully prepared via electroless plating method by using hydrazine hydrate (N2H4H2O) as a reducing agent. The coated powders were characterized with several techniques such as scanning electron microscope, energy dispersive spectrometer, Transmission electron microscopy, high-resolution transmission electron microscopy and X-ray diffraction to determine particle size, composition, phase and morphology. It indicated that the core–shell structure of Ni/Si3N4 has been constructed in the present method, the Ni layer on the surface of Si3N4 particles was relatively continuous and uniform, but it is inevitable that only in very small area occurred the aggregation of Ni particles. In principle, the coated process was successful and expectable. # 2009 Elsevier Ltd and Techna Group S.r.l. All rights reserved. Keywords: A. Powders: chemical preparation; B. Composites; C. Microstructure; D. Si3N4
2. Experimental procedure
Silicon nitride (Si3N4) ceramics have been investigated for many years for their potential application as structural materials because of their excellent mechanical properties at room and elevated temperatures. The wide use of Si3N4, however, is still limited due to its catastrophic fracture. By combining ceramic with metal homogeneously, materials with high fracture toughness can be achieved. Nickel (Ni), with excellent corrosion-resistance and wear-resistance properties, could be used as a ductile phase to improve toughness of brittle Si3N4. In recent years, various coating methods [1–4] have been developed to substitute the admixture method, by which the uniformity of the components can be improved, leading to the improvements of the sintering property and the stability of materials [5,6]. The electroless plating is one of the most effective coating techniques and could be applied on almost all material surfaces, such as plastic , ceramic [8–11], alloy  and powders [13,14]. In the present work, the Ni-coated Si3N4 powders were prepared via the electroless plating.
2.1. Preparation of the Si3N4
* Corresponding author. Tel.: +86 532 66781690; fax: +86 532 66781320. E-mail address: [email protected]
The Si3N4 powders (SN-E10, UBE, Japan, d50 = 0.3 mm) were used in the present study. Non-metallic material surface must have pretreatment process before electroless plating. In this work, the Si3N4 powders were processed as follows. Surface cleaning: to eliminate the impurities on original surface, the powers were immersed in hydrochloric acid for 10 min. Powers were then rinsed in deionized (DI) water until pH 7, then rinsed in ethanol. Etching: chemical roughening provides areas into which the deposited nickel became anchored and, therefore, roughening the surface typically improved adhesion. The coarse surface was gained at room temperature for 20 min by immersing in a solution of HF (concentration: 40% 20 ml/L), NH4F (2 g/L) and DI water. Activation: the Si3N4 powders surface was non-conducting, so the activation was necessary to improve its catalytic nature. Traditional palladium activation was introduced in this work. The etched powders were immersed at room temperature for 20 min in a palladium activation solution consisting of palladium chloride, PdCl2 (0.5 g/L), stannous chloride, SnCl22H2O (30 g/L), sodium chloride, NaCl (160 g/L) and hydrochloric acid, HCl (60 ml/L).
0272-8842/$36.00 # 2009 Elsevier Ltd and Techna Group S.r.l. All rights reserved. doi:10.1016/j.ceramint.2009.06.007
J. Dai et al. / Ceramics International 35 (2009) 3407–3410
Fig. 1. XRD patterns of the Ni/Si3N4 coated powders obtained at the different contents of NiCl2.
2.2. Electroless plating process The Si3N4 powders were then dispersed in DI water to form a Si3N4 suspension (Si3N4 concentration of 0.045 mol/l) via a 12 h stirring, and adjust pH value to 11 by adding NaOH solution. Then the coating was done with constant temperature baths (70 8C) having nickel chloride hexahydrate (NiCl26H2O) as the source of nickel and hydrazine hydrate (N2H4H2O) as the reducing agent. The NiCl2 solution and N2H4 solution were dropped into the suspension (the ratio of N2H4 to NiCl2 kept to be 7:1) and a 5 min stirring was performed. During the reaction process, the pH value of the system was kept constant by adding NaOH solution. After coating, the powers were centrifugalized, rinsed and dried.
Fig. 2. SEM morphologies of the (a) as-received Si3N4 powders, and (b) the Ni/ Si3N4 coated powders.
Fig. 3. SEM morphologies of the coated powders and element distribution of the surface from EDS: (b) N, (c) Si and (d) Ni.
J. Dai et al. / Ceramics International 35 (2009) 3407–3410
2.3. Characterization The phase composition was determined by X-ray diffraction (XRD). The morphology and composition of the coated powders were characterized by scanning electron microscope (SEM), Transmission electron microscopy (TEM), highresolution transmission electron microscopy (HRTEM) and energy dispersive spectrometer (EDS). 3. Results and discussion The phase composition of the coated powders was showed in Fig. 1. Only the two phases of Ni and Si3N4 were present in this experiment, indicating we can get Ni in the bath, and the quantity of Ni can be controlled through the quantity of NiCl2, so we can control the thickness of coated layer through the quantity of NiCl2 theoretically too. SEM micrographs of as-received Si3N4 powders and the Nicoated Si3N4 powders were presented in Fig. 2. The morphology seen in Fig. 2(a) was as-received Si3N4 powders with irregular shape, the surface was smooth in principle. In Fig. 2(b), all the Si3N4 powders were observed to be uniformly coated by the present electroless method and the coated Si3N4 powers retain their original high aspect ratio by this technique. In connection with the XRD analysis (Fig. 1), the layer is identified as Ni. In order to clarify the Ni and Si3N4 distribution in the coated powders, Si, N and Ni element distribution maps were obtained via EDS surface analysis and shown in Fig. 3 from the maps, it can be seen that the Ni element distribution was similar to that of the coated Si3N4 powders, indicating a successful coating process of Ni onto the Si3N4 particle surface. The Ni/Si3N4 composite microspheres were further investigated by TEM. Fig. 4 showed the TEM image of the microsphere. It is obviously shown that the Ni particles could
Fig. 4. TEM morphologies of the coated powders.
be dispersed on the surface of Si3N4 uniformly basically. However, a small darker area could be seen in Fig. 4, indicating Ni particles were aggregated in this area. As we know, segregation in small area in bath was inevitable. To identify the microstructure between the dark area and other area, HRTEM images which were taken of Fig. 4 as marked with boxes-and-arrow were observed. Fig. 5 shows the HRTEM of (a) dark area, (b) other area, and EDS profiles of (c) dark area and (d) other area. The EDS data in Fig. 5(c) and (d) confirmed that the elements of the selected area were Ni, N and Si without any other impurities. The singlet of O is probably from unavoidable surface-adsorption of oxygen on to the sample from exposure to air during sample processing. The atomic concentration of Ni in (c) and (d) was 5.28% and 1.83%. It confirmed that the concentration of Ni in dark area is higher than that of other area. Meanwhile, from the HRTEM image shown in Fig. 5(a) and (b), it was confirmed the core–shell
Fig. 5. HRTEM images of (a), (b), the (a), and (b) area in Fig. 4 and (c), and (d) their corresponding EDS profiles respectively.
J. Dai et al. / Ceramics International 35 (2009) 3407–3410
structure of the composites. On the particles surface of (a) and (b), the lattice spacing of 0.216 nm and 0.217 nm is observed respectively and this value is assigned to the (1 1 1) plane of Ni; in particles inner, the spacing of 0.224 (a) and 0.385 (b) corresponds to the (2 1 1) plane and (1 0 2) plane of Si3N4. The thickness of Ni shell in (a) and (b) is about 5 nm and 2 nm respectively, indicating the difference between these two areas. 4. Conclusion Through the processes of Surface cleaning, etching and activation, nickel film via electroless plating was deposited on the surface of Si3N4 successfully. The core–shell structure with shell of Ni and core of Si3N4 has been constructed. The Ni layer on the surface of Si3N4 particles was relatively continuous and uniform, only in very small area occurred the concentration of Ni particles. The thickness of Ni shell is about 2–5 nm. The preferable pH value is 11 and temperature is 70 8C for the reaction system. Acknowledgement This work was funded by the Natural Science Foundation of Shandong Province of China (Grant No. Y2006F47). References  Jae-kil Han, Fumio Saito, Byong-Taek Lee, Synthesis and characterization of nano-Ag spot-coated polymethylmethacrylate power by hydrothermalassisted attachment method, Mater. Lett. 61 (2007) 4177–4180.
 R. Zhang, L. Gao, J.K. Guo, Preparation and characterization of coated nanoscale Cu/SiCp composite particles, Ceram. Int. 30 (2004) 401–404.  S. Schaefers, L. Rast, A. Stanishevsky, Electroless silver plating on spincoated silver nanoparticle seed layers, Mater. Lett. 60 (2006) 706–709.  C.M. Das, P.K. Limaye, A.K. Grover, A.K. Suri, Preparation and characterization of silicon nitride codeposited electroless nickel composite coating, J. Alloys. Compd. 436 (2007) 328–334.  Keiichiro Tohgo, Takafumi Suzuki, Hiroyasu, Evaluation of R-curve behaviors of ceramic-metal functionally graded materials by stable crack growth, Araki, Eng. Fracture Mech. 72 (2005) 2359–2372.  W.H. Tuan, H.H. Wu, T.J. Yang, Preparation of Al2O3/Ni composites by pressureless sintering in H2, Ceram. Int. 21 (1995) 221–225.  S. Kishimoto, N. Shinya, New fabrication method for metallic closed cellular materials containing polymers, Mater. Des. 22 (2001) 535–539.  Sh. Alirezaei, S.M. Monirvaghefi, M. Salehi, A. Saatchi, Effect of alumina content on surface morphology and hardness of Ni–P–Al2O3 (a) electroless composite coatings, Surf. Coat. Technol. 184 (2004) 170–175.  Dai. Hongbin, Li. Hongxi, Wang. Fuhui, An alternative process for the preparation of Cu-coated mica composite powder, Surf. Coat. Technol. 201 (2006) 2859–2866.  Libo Li, Maozhong An, Electroless nickel-phosphorus plating on SiCp/Al composite from acid bath with nickel activation, 461 (2008) 85–91.  A.H.M. Esfakur Rahman, Jong-Hee Kim, Kap-Ho Lee, Byong-Taek Lee, Microstructure characterization and electrical conductivity of electroless nano Ni coated 8YSZ cermets, Surf. Coat. Technol. 202 (2008) 2182– 2188.  B. Szczygieł, A. Turkiewicz, J. Serafin´czuk, Surface morphology and structure of Ni–P, Ni–P–ZrO2, Ni–W–P, Ni–W–P–ZrO2, Surf. Coat. Technol. 202 (2008) 1904–1910.  A. Ozols, M. Pagnola, D. In˜aki Garcı´a, H. Sirkin, Electroless coating of permalloy powder and DC-resistivity of alloy composites, Surf. Coat. Technol. 200 (2006) 6821–6825.  H.B. Dai, H.X. Li, F.H. Wang, Electroless Ni–P coating preparation of conductive mica powder by a modified activation process, Appl. Surf. Sci. 253 (2006) 2474–2480.